#------------------------------------------------------------------------------
#$Date: 2021-03-23 10:34:38 +0200 (Tue, 23 Mar 2021) $
#$Revision: 263243 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/11/1561198.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1561198
loop_
_publ_author_name
'Xiao, Li-Na'
'Zhang, Hao'
'Zhang, Ting-Ting'
'Zhang, Xiao'
'Cui, Xiao-Bing'
_publ_section_title
;
 Two new POMOF compounds constructed from polyoxoanions, metals and
 organic ligands
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              11
_journal_page_last               18
_journal_paper_doi               10.1016/j.jssc.2017.12.025
_journal_volume                  259
_journal_year                    2018
_chemical_formula_sum            'C36 H36 Cu3 Mo12 N8 O42 P V2'
_chemical_formula_weight         2727.48
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_atom_sites_solution_hydrogens   geom
_cell_angle_alpha                98.64(3)
_cell_angle_beta                 99.090(17)
_cell_angle_gamma                100.40(3)
_cell_formula_units_Z            1
_cell_length_a                   10.826(4)
_cell_length_b                   10.876(2)
_cell_length_c                   13.584(3)
_cell_measurement_reflns_used    24429
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.55
_cell_measurement_theta_min      3.02
_cell_volume                     1526.9(8)
_computing_cell_refinement       'Bruker XSCANS'
_computing_data_collection       'Bruker XSCANS'
_computing_data_reduction        'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_molecular_graphics    'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_publication_material  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.992
_diffrn_measured_fraction_theta_max 0.980
_diffrn_measurement_device_type  'Bruker P4'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0265
_diffrn_reflns_av_unetI/netI     0.0351
_diffrn_reflns_Laue_measured_fraction_full 0.992
_diffrn_reflns_Laue_measured_fraction_max 0.980
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            14776
_diffrn_reflns_point_group_measured_fraction_full 0.992
_diffrn_reflns_point_group_measured_fraction_max 0.980
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.485
_diffrn_reflns_theta_min         3.022
_exptl_absorpt_coefficient_mu    3.819
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.6465
_exptl_absorpt_correction_type   empirical
_exptl_crystal_colour            dark
_exptl_crystal_density_diffrn    2.966
_exptl_crystal_description       block
_exptl_crystal_F_000             1296
_exptl_crystal_size_max          0.356
_exptl_crystal_size_mid          0.205
_exptl_crystal_size_min          0.147
_refine_diff_density_max         2.511
_refine_diff_density_min         -3.371
_refine_diff_density_rms         0.310
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.044
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     520
_refine_ls_number_reflns         6844
_refine_ls_number_restraints     510
_refine_ls_restrained_S_all      1.061
_refine_ls_R_factor_all          0.0699
_refine_ls_R_factor_gt           0.0642
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.1294P)²+21.3663P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1974
_refine_ls_wR_factor_ref         0.2036
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                6068
_reflns_number_total             6844
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            mmc2.cif
_cod_data_source_block           k1
_cod_original_cell_volume        1526.9(7)
_cod_database_code               1561198
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.79665(9) 0.42422(9) 0.17903(7) 0.0346(2) Uani 1 1 d . . . . .
Mo2 Mo 0.82491(7) 0.72163(6) 0.10216(6) 0.02110(19) Uani 1 1 d . . . . .
Mo3 Mo 0.96792(6) 0.19931(6) 0.08463(5) 0.01477(18) Uani 1 1 d . . . . .
Mo4 Mo 0.66019(6) 0.42060(7) -0.07288(7) 0.0253(2) Uani 1 1 d . . . . .
Mo5 Mo 1.13201(7) 0.50509(7) 0.25797(5) 0.02222(19) Uani 1 1 d . . . . .
Mo6 Mo 1.16063(9) 0.79633(8) 0.16974(7) 0.0323(2) Uani 1 1 d . . . . .
N1 N 0.6327(10) 0.5918(9) 0.4368(8) 0.044(2) Uani 1 1 d . . . . .
C1 C 0.5917(12) 0.6310(10) 0.3495(9) 0.045(3) Uani 1 1 d . . . . .
H1A H 0.5646 0.5715 0.2896 0.054 Uiso 1 1 calc R U . . .
C2 C 0.5890(12) 0.7569(10) 0.3472(8) 0.042(3) Uani 1 1 d . . . . .
H2A H 0.5613 0.7808 0.2859 0.050 Uiso 1 1 calc R U . . .
C3 C 0.6274(8) 0.8489(8) 0.4359(6) 0.0243(17) Uani 1 1 d . . . . .
C4 C 0.6270(8) 0.9846(8) 0.4356(6) 0.0236(16) Uani 1 1 d . . . . .
C5 C 0.5555(11) 1.0255(10) 0.3571(8) 0.039(2) Uani 1 1 d . . . . .
H5A H 0.5042 0.9655 0.3034 0.047 Uiso 1 1 calc R U . . .
C6 C 0.5590(14) 1.1515(11) 0.3572(9) 0.049(3) Uani 1 1 d . . . . .
H6A H 0.5093 1.1749 0.3037 0.059 Uiso 1 1 calc R U . . .
N2 N 0.6320(9) 1.2431(8) 0.4324(8) 0.040(2) Uani 1 1 d . . . . .
C7 C 0.6965(10) 1.2045(9) 0.5116(9) 0.038(2) Uani 1 1 d . . . . .
H7A H 0.7433 1.2656 0.5665 0.046 Uiso 1 1 calc R U . . .
C8 C 0.6957(10) 1.0801(9) 0.5143(7) 0.032(2) Uani 1 1 d . . . . .
H8A H 0.7425 1.0586 0.5704 0.038 Uiso 1 1 calc R U . . .
C9 C 0.6690(10) 0.8071(10) 0.5244(7) 0.035(2) Uani 1 1 d . . . . .
H9A H 0.6962 0.8648 0.5853 0.042 Uiso 1 1 calc R U . . .
C10 C 0.6700(12) 0.6796(10) 0.5222(8) 0.041(2) Uani 1 1 d . . . . .
H10A H 0.6977 0.6537 0.5826 0.049 Uiso 1 1 calc R U . . .
V1 V 0.74262(12) 0.68210(12) -0.13345(11) 0.0204(3) Uani 1 1 d . . . . .
P1 P 1.0000 0.5000 0.0000 0.0089(4) Uani 1 2 d S . P . .
O1 O 1.1135(9) 0.5671(10) 0.0909(8) 0.0137(18) Uani 0.5 1 d . U P . .
O2 O 0.9840(10) 0.4319(10) 0.0884(8) 0.0151(18) Uani 0.5 1 d . U P . .
O3 O 0.9998(10) 0.6403(9) 0.0272(8) 0.0158(18) Uani 0.5 1 d . U P . .
O4 O 0.8746(10) 0.5166(10) 0.0371(8) 0.0163(18) Uani 0.5 1 d . U P . .
O5 O 0.8455(7) 0.2637(8) 0.1412(7) 0.0480(19) Uani 1 1 d . U . . .
O6 O 0.9846(7) 0.7954(9) 0.1717(5) 0.0431(17) Uani 1 1 d . U . . .
O7 O 1.1996(8) 0.5046(7) 0.3781(5) 0.0409(18) Uani 1 1 d . U . . .
O8 O 0.8671(6) 0.1486(9) -0.0411(5) 0.0448(18) Uani 1 1 d . U . . .
O9 O 0.9617(7) 0.0653(7) 0.1280(7) 0.048(2) Uani 1 1 d . U . . .
O10 O 0.7086(8) 0.3911(7) 0.2632(6) 0.0420(19) Uani 1 1 d . U . . .
O11 O 0.6414(7) 0.7520(7) -0.1876(7) 0.047(2) Uani 1 1 d . U . . .
O12 O 0.7939(9) 0.5992(7) 0.1782(6) 0.052(2) Uani 1 1 d . U . . .
O13 O 0.9640(7) 0.4780(8) 0.2664(7) 0.0490(19) Uani 1 1 d . U . . .
O14 O 0.8720(6) 0.7890(7) -0.0234(5) 0.0328(14) Uani 1 1 d . U . . .
O15 O 1.2340(7) 0.9275(7) 0.2461(5) 0.0379(17) Uani 1 1 d . U . . .
O16 O 0.7419(8) 0.8263(8) 0.1442(6) 0.0436(18) Uani 1 1 d . U . . .
O17 O 0.6984(8) 0.6095(6) -0.0183(6) 0.0410(17) Uani 1 1 d . U . . .
O18 O 1.1057(6) 0.3178(6) 0.1944(5) 0.0302(13) Uani 1 1 d . U . . .
O19 O 0.7175(8) 0.5013(6) -0.1880(7) 0.0410(16) Uani 1 1 d . U . . .
O20 O 0.5041(6) 0.3917(6) -0.1134(5) 0.0296(14) Uani 1 1 d . U . . .
O21 O 0.7014(9) 0.2727(8) -0.1255(8) 0.056(2) Uani 1 1 d . U . . .
O22 O 1.1514(9) 0.6735(8) 0.2583(7) 0.0495(18) Uani 1 1 d . U . . .
O23 O 0.6783(9) 0.3848(7) 0.0530(7) 0.057(2) Uani 1 1 d . U . . .
Cu1 Cu 0.64165(18) 0.41897(14) 0.43124(17) 0.0626(5) Uani 1 1 d . . . . .
Cu2 Cu 1.0094(10) 0.5044(8) 0.5188(3) 0.0380(12) Uani 0.5 1 d . . P . .
C13 C 0.9956(9) 0.9327(7) 0.5012(6) 0.0236(17) Uani 1 1 d . . . . .
C12 C 0.9589(10) 0.8398(9) 0.4143(7) 0.0306(19) Uani 1 1 d . . . . .
H12A H 0.9338 0.8636 0.3525 0.037 Uiso 1 1 calc R U . . .
N3 N 0.9921(9) 0.6743(8) 0.5042(8) 0.043(2) Uani 1 1 d . . . . .
C11 C 0.9582(10) 0.7172(9) 0.4162(9) 0.038(2) Uani 1 1 d . . . . .
H11A H 0.9338 0.6589 0.3555 0.045 Uiso 1 1 calc R U . . .
C15 C 1.0242(12) 0.7593(10) 0.5897(9) 0.042(3) Uani 1 1 d . . . . .
H15A H 1.0455 0.7317 0.6505 0.050 Uiso 1 1 calc R U . . .
C14 C 1.0272(12) 0.8881(9) 0.5918(8) 0.038(2) Uani 1 1 d . . . . .
H14A H 1.0502 0.9448 0.6533 0.045 Uiso 1 1 calc R U . . .
N4 N 0.5917(6) 0.0880(6) -0.0010(6) 0.0201(13) Uani 1 1 d . . . . .
C16 C 0.5227(19) 0.0304(19) -0.1068(14) 0.031(4) Uani 0.5 1 d . . P . .
C17 C 0.6148(17) -0.0342(15) -0.0604(17) 0.030(4) Uani 0.5 1 d . . P . .
C18 C 0.6405(16) -0.0071(17) 0.0511(16) 0.029(4) Uani 0.5 1 d . . P . .
C19 C 0.5931(19) 0.0716(18) 0.1064(15) 0.032(4) Uani 0.5 1 d . . P . .
C20 C 0.4955(15) 0.1442(15) 0.0533(14) 0.023(3) Uani 0.5 1 d . . P . .
C21 C 0.4715(17) 0.1182(16) -0.0459(16) 0.029(4) Uani 0.5 1 d . . P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O10 Mo1 O23 104.5(5) . .
O10 Mo1 O12 102.3(4) . .
O23 Mo1 O12 87.5(3) . .
O10 Mo1 O5 101.5(4) . .
O23 Mo1 O5 87.7(4) . .
O12 Mo1 O5 156.2(4) . .
O10 Mo1 O13 99.9(4) . .
O23 Mo1 O13 155.6(4) . .
O12 Mo1 O13 88.5(4) . .
O5 Mo1 O13 86.2(3) . .
O10 Mo1 O4 160.7(4) . .
O23 Mo1 O4 64.4(4) . .
O12 Mo1 O4 62.9(4) . .
O5 Mo1 O4 94.1(4) . .
O13 Mo1 O4 92.5(4) . .
O16 Mo2 O6 101.1(4) . .
O16 Mo2 O12 102.5(4) . .
O6 Mo2 O12 96.6(4) . .
O16 Mo2 O17 102.5(4) . .
O6 Mo2 O17 153.4(4) . .
O12 Mo2 O17 90.1(3) . .
O16 Mo2 O14 100.9(4) . .
O6 Mo2 O14 89.3(3) . .
O12 Mo2 O14 154.3(4) . .
O17 Mo2 O14 74.4(3) . .
O16 Mo2 O4 159.6(4) . .
O6 Mo2 O4 96.3(4) . .
O12 Mo2 O4 64.8(4) . .
O17 Mo2 O4 63.4(3) . .
O14 Mo2 O4 89.7(3) . .
O16 Mo2 O3 158.1(4) . .
O6 Mo2 O3 66.1(4) . .
O12 Mo2 O3 96.7(4) . .
O17 Mo2 O3 87.6(4) . .
O14 Mo2 O3 62.8(3) . .
O4 Mo2 O3 41.6(3) . .
O16 Mo2 V1 103.3(3) . .
O6 Mo2 V1 124.3(2) . .
O12 Mo2 V1 125.1(2) . .
O17 Mo2 V1 37.1(2) . .
O14 Mo2 V1 37.32(18) . .
O4 Mo2 V1 74.8(3) . .
O3 Mo2 V1 73.2(3) . .
O9 Mo3 O8 102.8(4) . .
O9 Mo3 O5 101.2(5) . .
O8 Mo3 O5 93.9(4) . .
O9 Mo3 O14 102.1(4) . 2_765
O8 Mo3 O14 90.8(3) . 2_765
O5 Mo3 O14 154.6(4) . 2_765
O9 Mo3 O18 100.4(4) . .
O8 Mo3 O18 155.3(3) . .
O5 Mo3 O18 89.7(3) . .
O14 Mo3 O18 76.1(3) 2_765 .
O9 Mo3 O3 161.1(4) . 2_765
O8 Mo3 O3 66.9(4) . 2_765
O5 Mo3 O3 95.5(4) . 2_765
O14 Mo3 O3 63.6(3) 2_765 2_765
O18 Mo3 O3 88.5(3) . 2_765
O9 Mo3 O2 158.4(4) . .
O8 Mo3 O2 95.6(4) . .
O5 Mo3 O2 66.0(4) . .
O14 Mo3 O2 88.8(3) 2_765 .
O18 Mo3 O2 63.8(3) . .
O3 Mo3 O2 39.8(3) 2_765 .
O9 Mo3 V1 102.6(3) . 2_765
O8 Mo3 V1 126.5(2) . 2_765
O5 Mo3 V1 125.6(2) . 2_765
O14 Mo3 V1 37.94(18) 2_765 2_765
O18 Mo3 V1 38.21(18) . 2_765
O3 Mo3 V1 74.1(2) 2_765 2_765
O2 Mo3 V1 74.5(2) . 2_765
O20 Mo4 O23 104.3(4) . .
O20 Mo4 O21 102.3(4) . .
O23 Mo4 O21 92.6(4) . .
O20 Mo4 O17 101.5(3) . .
O23 Mo4 O17 91.8(3) . .
O21 Mo4 O17 153.9(4) . .
O20 Mo4 O19 99.0(3) . .
O23 Mo4 O19 155.3(4) . .
O21 Mo4 O19 90.2(3) . .
O17 Mo4 O19 75.6(3) . .
O20 Mo4 O1 155.4(3) . 2_765
O23 Mo4 O1 96.8(4) . 2_765
O21 Mo4 O1 63.7(4) . 2_765
O17 Mo4 O1 90.2(3) . 2_765
O19 Mo4 O1 62.7(3) . 2_765
O20 Mo4 O4 159.4(3) . .
O23 Mo4 O4 65.4(4) . .
O21 Mo4 O4 96.2(4) . .
O17 Mo4 O4 62.6(3) . .
O19 Mo4 O4 89.9(3) . .
O1 Mo4 O4 44.1(3) 2_765 .
O20 Mo4 V1 101.1(2) . .
O23 Mo4 V1 127.3(2) . .
O21 Mo4 V1 125.8(2) . .
O17 Mo4 V1 37.7(2) . .
O19 Mo4 V1 38.0(2) . .
O1 Mo4 V1 75.2(2) 2_765 .
O4 Mo4 V1 74.8(2) . .
O7 Mo5 O22 101.3(4) . .
O7 Mo5 O13 100.9(4) . .
O22 Mo5 O13 96.0(4) . .
O7 Mo5 O19 100.9(4) . 2_765
O22 Mo5 O19 90.5(3) . 2_765
O13 Mo5 O19 155.5(4) . 2_765
O7 Mo5 O18 101.2(3) . .
O22 Mo5 O18 155.7(4) . .
O13 Mo5 O18 88.6(3) . .
O19 Mo5 O18 76.3(3) 2_765 .
O7 Mo5 O1 157.1(4) . .
O22 Mo5 O1 64.2(4) . .
O13 Mo5 O1 98.3(4) . .
O19 Mo5 O1 63.5(3) 2_765 .
O18 Mo5 O1 91.5(3) . .
O7 Mo5 O2 159.1(4) . .
O22 Mo5 O2 96.7(4) . .
O13 Mo5 O2 66.5(3) . .
O19 Mo5 O2 89.3(4) 2_765 .
O18 Mo5 O2 63.3(3) . .
O1 Mo5 O2 43.3(3) . .
O7 Mo5 V1 102.7(3) . 2_765
O22 Mo5 V1 126.3(2) . 2_765
O13 Mo5 V1 125.0(2) . 2_765
O19 Mo5 V1 38.1(2) 2_765 2_765
O18 Mo5 V1 38.31(18) . 2_765
O1 Mo5 V1 75.7(2) . 2_765
O2 Mo5 V1 74.3(2) . 2_765
O15 Mo6 O6 103.2(4) . .
O15 Mo6 O21 103.1(4) . 2_765
O6 Mo6 O21 153.7(4) . 2_765
O15 Mo6 O8 102.1(4) . 2_765
O6 Mo6 O8 87.0(3) . 2_765
O21 Mo6 O8 87.1(4) 2_765 2_765
O15 Mo6 O22 103.0(4) . .
O6 Mo6 O22 87.7(4) . .
O21 Mo6 O22 86.9(3) 2_765 .
O8 Mo6 O22 154.9(4) 2_765 .
O15 Mo6 O1 158.3(4) . .
O6 Mo6 O1 92.4(3) . .
O21 Mo6 O1 62.4(4) 2_765 .
O8 Mo6 O1 93.6(4) 2_765 .
O22 Mo6 O1 62.1(4) . .
C10 N1 C1 117.8(9) . .
C10 N1 Cu1 123.4(8) . .
C1 N1 Cu1 118.7(8) . .
N1 C1 C2 121.8(10) . .
N1 C1 H1A 119.1 . .
C2 C1 H1A 119.1 . .
C1 C2 C3 120.8(10) . .
C1 C2 H2A 119.6 . .
C3 C2 H2A 119.6 . .
C9 C3 C2 116.7(9) . .
C9 C3 C4 121.3(8) . .
C2 C3 C4 122.0(8) . .
C8 C4 C5 115.1(8) . .
C8 C4 C3 122.3(8) . .
C5 C4 C3 122.5(8) . .
C6 C5 C4 121.5(10) . .
C6 C5 H5A 119.2 . .
C4 C5 H5A 119.2 . .
N2 C6 C5 122.2(10) . .
N2 C6 H6A 118.9 . .
C5 C6 H6A 118.9 . .
C6 N2 C7 116.8(9) . .
C6 N2 Cu1 122.5(8) . 1_565
C7 N2 Cu1 120.6(7) . 1_565
N2 C7 C8 122.7(9) . .
N2 C7 H7A 118.7 . .
C8 C7 H7A 118.7 . .
C7 C8 C4 121.5(9) . .
C7 C8 H8A 119.3 . .
C4 C8 H8A 119.3 . .
C10 C9 C3 120.0(9) . .
C10 C9 H9A 120.0 . .
C3 C9 H9A 120.0 . .
N1 C10 C9 122.9(10) . .
N1 C10 H10A 118.5 . .
C9 C10 H10A 118.5 . .
O11 V1 O17 116.3(4) . .
O11 V1 O14 115.5(4) . .
O17 V1 O14 79.0(3) . .
O11 V1 O19 114.7(4) . .
O17 V1 O19 79.3(3) . .
O14 V1 O19 129.8(4) . .
O11 V1 O18 114.2(4) . 2_765
O17 V1 O18 129.6(4) . 2_765
O14 V1 O18 80.0(3) . 2_765
O19 V1 O18 80.0(3) . 2_765
O11 V1 Mo5 121.2(4) . 2_765
O17 V1 Mo5 108.0(3) . 2_765
O14 V1 Mo5 109.0(2) . 2_765
O19 V1 Mo5 39.7(2) . 2_765
O18 V1 Mo5 40.38(19) 2_765 2_765
O11 V1 Mo3 121.5(3) . 2_765
O17 V1 Mo3 108.2(2) . 2_765
O14 V1 Mo3 39.96(19) . 2_765
O19 V1 Mo3 109.1(2) . 2_765
O18 V1 Mo3 40.10(18) 2_765 2_765
Mo5 V1 Mo3 74.40(5) 2_765 2_765
O11 V1 Mo4 121.8(3) . .
O17 V1 Mo4 39.5(2) . .
O14 V1 Mo4 108.4(2) . .
O19 V1 Mo4 39.9(2) . .
O18 V1 Mo4 109.2(2) 2_765 .
Mo5 V1 Mo4 73.78(4) 2_765 .
Mo3 V1 Mo4 116.66(5) 2_765 .
O11 V1 Mo2 122.9(4) . .
O17 V1 Mo2 39.2(2) . .
O14 V1 Mo2 39.9(2) . .
O19 V1 Mo2 108.1(3) . .
O18 V1 Mo2 108.9(2) 2_765 .
Mo5 V1 Mo2 115.91(5) 2_765 .
Mo3 V1 Mo2 73.91(4) 2_765 .
Mo4 V1 Mo2 73.23(5) . .
O3 P1 O3 180.0 . 2_765
O3 P1 O2 112.0(6) . .
O3 P1 O2 68.0(6) 2_765 .
O3 P1 O2 68.0(6) . 2_765
O3 P1 O2 112.0(6) 2_765 2_765
O2 P1 O2 180.0 . 2_765
O3 P1 O4 70.3(6) . .
O3 P1 O4 109.7(6) 2_765 .
O2 P1 O4 69.5(6) . .
O2 P1 O4 110.5(6) 2_765 .
O3 P1 O4 109.7(6) . 2_765
O3 P1 O4 70.3(6) 2_765 2_765
O2 P1 O4 110.5(6) . 2_765
O2 P1 O4 69.5(6) 2_765 2_765
O4 P1 O4 180.0 . 2_765
O3 P1 O1 110.4(5) . 2_765
O3 P1 O1 69.6(5) 2_765 2_765
O2 P1 O1 107.6(6) . 2_765
O2 P1 O1 72.4(6) 2_765 2_765
O4 P1 O1 73.4(5) . 2_765
O4 P1 O1 106.6(5) 2_765 2_765
O3 P1 O1 69.6(5) . .
O3 P1 O1 110.4(5) 2_765 .
O2 P1 O1 72.4(6) . .
O2 P1 O1 107.6(6) 2_765 .
O4 P1 O1 106.6(5) . .
O4 P1 O1 73.4(5) 2_765 .
O1 P1 O1 180.0 2_765 .
P1 O1 O3 53.5(5) . .
P1 O1 Mo5 122.4(5) . .
O3 O1 Mo5 130.5(6) . .
P1 O1 Mo4 121.1(5) . 2_765
O3 O1 Mo4 127.7(6) . 2_765
Mo5 O1 Mo4 97.6(3) . 2_765
P1 O1 Mo6 125.1(5) . .
O3 O1 Mo6 71.6(5) . .
Mo5 O1 Mo6 91.3(3) . .
Mo4 O1 Mo6 91.1(3) 2_765 .
P1 O2 O3 55.9(5) . 2_765
P1 O2 O4 56.1(5) . .
O3 O2 O4 93.3(7) 2_765 .
P1 O2 Mo3 125.9(6) . .
O3 O2 Mo3 70.0(5) 2_765 .
O4 O2 Mo3 131.3(6) . .
P1 O2 Mo5 121.7(6) . .
O3 O2 Mo5 134.0(6) 2_765 .
O4 O2 Mo5 124.5(6) . .
Mo3 O2 Mo5 96.4(3) . .
P1 O3 O2 56.1(5) . 2_765
P1 O3 O4 55.8(5) . .
O2 O3 O4 93.5(7) 2_765 .
P1 O3 O1 56.9(5) . .
O2 O3 O1 92.3(7) 2_765 .
O4 O3 O1 90.5(7) . .
P1 O3 Mo3 126.3(6) . 2_765
O2 O3 Mo3 70.2(5) 2_765 2_765
O4 O3 Mo3 136.4(7) . 2_765
O1 O3 Mo3 129.0(6) . 2_765
P1 O3 Mo2 123.0(6) . .
O2 O3 Mo2 136.3(7) 2_765 .
O4 O3 Mo2 67.3(5) . .
O1 O3 Mo2 125.0(6) . .
Mo3 O3 Mo2 96.4(3) 2_765 .
P1 O4 O2 54.4(5) . .
P1 O4 O3 53.9(5) . .
O2 O4 O3 91.4(7) . .
P1 O4 Mo2 124.9(6) . .
O2 O4 Mo2 131.6(7) . .
O3 O4 Mo2 71.1(5) . .
P1 O4 Mo1 125.0(6) . .
O2 O4 Mo1 70.6(5) . .
O3 O4 Mo1 135.5(7) . .
Mo2 O4 Mo1 90.6(3) . .
P1 O4 Mo4 121.2(6) . .
O2 O4 Mo4 125.7(6) . .
O3 O4 Mo4 132.4(7) . .
Mo2 O4 Mo4 96.8(4) . .
Mo1 O4 Mo4 88.8(3) . .
Mo3 O5 Mo1 140.4(5) . .
Mo2 O6 Mo6 142.0(5) . .
Mo3 O8 Mo6 140.1(5) . 2_765
Mo2 O12 Mo1 141.5(6) . .
Mo5 O13 Mo1 139.9(5) . .
V1 O14 Mo3 102.1(3) . 2_765
V1 O14 Mo2 102.8(3) . .
Mo3 O14 Mo2 132.4(4) 2_765 .
V1 O17 Mo4 102.7(4) . .
V1 O17 Mo2 103.7(3) . .
Mo4 O17 Mo2 132.6(4) . .
V1 O18 Mo3 101.7(3) 2_765 .
V1 O18 Mo5 101.3(3) 2_765 .
Mo3 O18 Mo5 133.0(4) . .
V1 O19 Mo5 102.2(3) . 2_765
V1 O19 Mo4 102.1(4) . .
Mo5 O19 Mo4 132.9(4) 2_765 .
Mo4 O21 Mo6 142.6(5) . 2_765
Mo5 O22 Mo6 142.2(6) . .
Mo4 O23 Mo1 141.2(5) . .
N1 Cu1 N2 173.0(4) . 1_545
Cu2 Cu2 N3 83(2) 2_766 2_766
Cu2 Cu2 N3 82(2) 2_766 .
N3 Cu2 N3 164.8(2) 2_766 .
C12 C13 C14 115.2(8) . .
C12 C13 C13 122.5(10) . 2_776
C14 C13 C13 122.2(9) . 2_776
C11 C12 C13 122.3(10) . .
C11 C12 H12A 118.8 . .
C13 C12 H12A 118.8 . .
C15 N3 C11 117.4(8) . .
C15 N3 Cu2 130.1(9) . 2_766
C11 N3 Cu2 112.4(7) . 2_766
C15 N3 Cu2 114.9(8) . .
C11 N3 Cu2 127.5(7) . .
Cu2 N3 Cu2 15.2(2) 2_766 .
C12 C11 N3 122.4(9) . .
C12 C11 H11A 118.8 . .
N3 C11 H11A 118.8 . .
N3 C15 C14 122.4(10) . .
N3 C15 H15A 118.8 . .
C14 C15 H15A 118.8 . .
C15 C14 C13 120.2(9) . .
C15 C14 H14A 119.9 . .
C13 C14 H14A 119.9 . .
C21 N4 C18 141.0(10) . .
C21 N4 C19 111.3(12) . .
C18 N4 C19 51.4(12) . .
C21 N4 C16 57.2(11) . .
C18 N4 C16 111.3(12) . .
C19 N4 C16 141.3(11) . .
C21 N4 C17 111.6(12) . .
C18 N4 C17 58.8(12) . .
C19 N4 C17 108.1(12) . .
C16 N4 C17 56.8(11) . .
C21 N4 C20 51.8(11) . .
C18 N4 C20 111.1(11) . .
C19 N4 C20 62.9(11) . .
C16 N4 C20 106.4(11) . .
C17 N4 C20 143.7(10) . .
C21 C16 C17 120.1(17) . .
C21 C16 N4 60.3(11) . .
C17 C16 N4 62.8(11) . .
C21 C16 C19 88.8(15) . 2_655
C17 C16 C19 95.2(15) . 2_655
N4 C16 C19 110.9(14) . 2_655
C21 C16 C18 49.3(10) . 2_655
C17 C16 C18 112.8(14) . 2_655
N4 C16 C18 87.4(11) . 2_655
C19 C16 C18 39.4(11) 2_655 2_655
C16 C17 C18 114.3(15) . .
C16 C17 N4 60.4(10) . .
C18 C17 N4 58.5(10) . .
C16 C17 C20 90.0(14) . 2_655
C18 C17 C20 86.6(14) . 2_655
N4 C17 C20 107.1(12) . 2_655
C19 C18 N4 65.4(12) . .
C19 C18 C17 125.4(17) . .
N4 C18 C17 62.8(11) . .
C19 C18 C21 93.1(15) . 2_655
N4 C18 C21 108.3(13) . 2_655
C17 C18 C21 87.3(15) . 2_655
C19 C18 C16 48.7(12) . 2_655
N4 C18 C16 86.9(10) . 2_655
C17 C18 C16 111.7(13) . 2_655
C21 C18 C16 44.4(10) 2_655 2_655
C18 C19 N4 63.2(12) . .
C18 C19 C16 91.8(16) . 2_655
N4 C19 C16 107.5(14) . 2_655
C18 C19 C20 119.1(18) . .
N4 C19 C20 59.7(10) . .
C16 C19 C20 86.5(14) 2_655 .
C21 C20 N4 61.4(11) . .
C21 C20 C17 92.4(15) . 2_655
N4 C20 C17 108.9(11) . 2_655
C21 C20 C19 115.2(15) . .
N4 C20 C19 57.4(10) . .
C17 C20 C19 88.3(13) 2_655 .
C20 C21 C16 125.7(17) . .
C20 C21 N4 66.8(12) . .
C16 C21 N4 62.6(11) . .
C20 C21 C18 93.6(16) . 2_655
C16 C21 C18 86.3(14) . 2_655
N4 C21 C18 110.2(12) . 2_655
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mo1 O10 1.640(7) .
Mo1 O23 1.909(7) .
Mo1 O12 1.910(7) .
Mo1 O5 1.934(7) .
Mo1 O13 1.940(7) .
Mo1 O4 2.496(11) .
Mo2 O16 1.663(7) .
Mo2 O6 1.811(7) .
Mo2 O12 1.820(8) .
Mo2 O17 2.032(7) .
Mo2 O14 2.054(7) .
Mo2 O4 2.457(10) .
Mo2 O3 2.520(10) .
Mo2 V1 3.1255(18) .
Mo3 O9 1.646(6) .
Mo3 O8 1.823(7) .
Mo3 O5 1.825(7) .
Mo3 O14 2.030(7) 2_765
Mo3 O18 2.033(6) .
Mo3 O3 2.493(10) 2_765
Mo3 O2 2.496(10) .
Mo3 V1 3.0904(19) 2_765
Mo4 O20 1.649(6) .
Mo4 O23 1.799(8) .
Mo4 O21 1.820(8) .
Mo4 O17 2.020(7) .
Mo4 O19 2.031(7) .
Mo4 O1 2.482(10) 2_765
Mo4 O4 2.504(11) .
Mo4 V1 3.0954(16) .
Mo5 O7 1.680(7) .
Mo5 O22 1.804(8) .
Mo5 O13 1.814(8) .
Mo5 O19 2.018(7) 2_765
Mo5 O18 2.040(7) .
Mo5 O1 2.451(11) .
Mo5 O2 2.516(11) .
Mo5 V1 3.0881(19) 2_765
Mo6 O15 1.621(6) .
Mo6 O6 1.909(7) .
Mo6 O21 1.926(8) 2_765
Mo6 O8 1.927(8) 2_765
Mo6 O22 1.927(8) .
Mo6 O1 2.488(10) .
N1 C10 1.342(15) .
N1 C1 1.355(16) .
N1 Cu1 1.890(9) .
C1 C2 1.380(15) .
C1 H1A 0.9300 .
C2 C3 1.398(13) .
C2 H2A 0.9300 .
C3 C9 1.387(13) .
C3 C4 1.477(12) .
C4 C8 1.383(12) .
C4 C5 1.393(13) .
C5 C6 1.363(15) .
C5 H5A 0.9300 .
C6 N2 1.347(15) .
C6 H6A 0.9300 .
N2 C7 1.352(15) .
N2 Cu1 1.899(9) 1_565
C7 C8 1.358(14) .
C7 H7A 0.9300 .
C8 H8A 0.9300 .
C9 C10 1.384(14) .
C9 H9A 0.9300 .
C10 H10A 0.9300 .
V1 O11 1.591(7) .
V1 O17 1.942(8) .
V1 O14 1.943(7) .
V1 O19 1.948(7) .
V1 O18 1.952(6) 2_765
V1 Mo5 3.0881(19) 2_765
V1 Mo3 3.0905(19) 2_765
P1 O3 1.516(10) .
P1 O3 1.516(10) 2_765
P1 O2 1.519(10) .
P1 O2 1.519(10) 2_765
P1 O4 1.551(10) .
P1 O4 1.551(10) 2_765
P1 O1 1.579(10) 2_765
P1 O1 1.579(10) .
O1 O3 1.768(14) .
O1 Mo4 2.482(10) 2_765
O2 O3 1.697(15) 2_765
O2 O4 1.750(15) .
O3 O2 1.697(15) 2_765
O3 O4 1.767(15) .
O3 Mo3 2.493(10) 2_765
O8 Mo6 1.927(8) 2_765
O14 Mo3 2.030(7) 2_765
O18 V1 1.952(6) 2_765
O19 Mo5 2.018(7) 2_765
O21 Mo6 1.926(8) 2_765
Cu1 N2 1.899(9) 1_545
Cu2 Cu2 0.507(8) 2_766
Cu2 N3 1.919(12) 2_766
Cu2 N3 1.927(12) .
C13 C12 1.386(11) .
C13 C14 1.404(13) .
C13 C13 1.456(16) 2_776
C12 C11 1.336(14) .
C12 H12A 0.9300 .
N3 C15 1.325(15) .
N3 C11 1.368(16) .
N3 Cu2 1.919(12) 2_766
C11 H11A 0.9300 .
C15 C14 1.392(13) .
C15 H15A 0.9300 .
C14 H14A 0.9300 .
N4 C21 1.462(18) .
N4 C18 1.466(18) .
N4 C19 1.49(2) .
N4 C16 1.50(2) .
N4 C17 1.530(17) .
N4 C20 1.530(17) .
C16 C21 1.42(3) .
C16 C17 1.44(3) .
C16 C19 1.52(3) 2_655
C16 C18 2.02(3) 2_655
C17 C18 1.47(3) .
C17 C20 1.56(2) 2_655
C18 C19 1.28(3) .
C18 C21 1.53(2) 2_655
C18 C16 2.02(3) 2_655
C19 C16 1.52(3) 2_655
C19 C20 1.58(3) .
C20 C21 1.31(3) .
C20 C17 1.56(2) 2_655
C21 C18 1.53(2) 2_655
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
C10 N1 C1 C2 0.6(19) . . . .
Cu1 N1 C1 C2 -176.6(10) . . . .
N1 C1 C2 C3 -1(2) . . . .
C1 C2 C3 C9 0.7(17) . . . .
C1 C2 C3 C4 179.3(10) . . . .
C9 C3 C4 C8 16.6(14) . . . .
C2 C3 C4 C8 -161.8(10) . . . .
C9 C3 C4 C5 -162.0(10) . . . .
C2 C3 C4 C5 19.5(15) . . . .
C8 C4 C5 C6 2.9(17) . . . .
C3 C4 C5 C6 -178.4(11) . . . .
C4 C5 C6 N2 0(2) . . . .
C5 C6 N2 C7 -3.9(19) . . . .
C5 C6 N2 Cu1 178.0(10) . . . 1_565
C6 N2 C7 C8 4.0(16) . . . .
Cu1 N2 C7 C8 -177.9(8) 1_565 . . .
N2 C7 C8 C4 -0.6(16) . . . .
C5 C4 C8 C7 -2.8(15) . . . .
C3 C4 C8 C7 178.5(9) . . . .
C2 C3 C9 C10 -0.5(16) . . . .
C4 C3 C9 C10 -179.1(10) . . . .
C1 N1 C10 C9 -0.5(19) . . . .
Cu1 N1 C10 C9 176.7(9) . . . .
C3 C9 C10 N1 0.4(18) . . . .
O3 P1 O1 O3 179.999(2) 2_765 . . .
O2 P1 O1 O3 -122.5(6) . . . .
O2 P1 O1 O3 57.5(6) 2_765 . . .
O4 P1 O1 O3 -61.0(6) . . . .
O4 P1 O1 O3 119.0(6) 2_765 . . .
O3 P1 O1 Mo5 119.2(7) . . . .
O3 P1 O1 Mo5 -60.8(7) 2_765 . . .
O2 P1 O1 Mo5 -3.3(6) . . . .
O2 P1 O1 Mo5 176.7(6) 2_765 . . .
O4 P1 O1 Mo5 58.2(7) . . . .
O4 P1 O1 Mo5 -121.8(7) 2_765 . . .
O3 P1 O1 Mo4 -116.3(7) . . . 2_765
O3 P1 O1 Mo4 63.7(7) 2_765 . . 2_765
O2 P1 O1 Mo4 121.3(7) . . . 2_765
O2 P1 O1 Mo4 -58.7(7) 2_765 . . 2_765
O4 P1 O1 Mo4 -177.2(6) . . . 2_765
O4 P1 O1 Mo4 2.8(6) 2_765 . . 2_765
O3 P1 O1 Mo6 0.6(6) . . . .
O3 P1 O1 Mo6 -179.4(6) 2_765 . . .
O2 P1 O1 Mo6 -121.9(7) . . . .
O2 P1 O1 Mo6 58.1(7) 2_765 . . .
O4 P1 O1 Mo6 -60.4(7) . . . .
O4 P1 O1 Mo6 119.6(7) 2_765 . . .
O3 P1 O2 O3 180.001(1) . . . 2_765
O4 P1 O2 O3 122.6(7) . . . 2_765
O4 P1 O2 O3 -57.4(7) 2_765 . . 2_765
O1 P1 O2 O3 58.6(6) 2_765 . . 2_765
O1 P1 O2 O3 -121.4(6) . . . 2_765
O3 P1 O2 O4 57.4(7) . . . .
O3 P1 O2 O4 -122.6(7) 2_765 . . .
O4 P1 O2 O4 179.999(2) 2_765 . . .
O1 P1 O2 O4 -64.0(6) 2_765 . . .
O1 P1 O2 O4 116.0(6) . . . .
O3 P1 O2 Mo3 177.2(6) . . . .
O3 P1 O2 Mo3 -2.8(6) 2_765 . . .
O4 P1 O2 Mo3 119.8(8) . . . .
O4 P1 O2 Mo3 -60.2(8) 2_765 . . .
O1 P1 O2 Mo3 55.7(7) 2_765 . . .
O1 P1 O2 Mo3 -124.3(7) . . . .
O3 P1 O2 Mo5 -55.4(7) . . . .
O3 P1 O2 Mo5 124.6(7) 2_765 . . .
O4 P1 O2 Mo5 -112.8(7) . . . .
O4 P1 O2 Mo5 67.2(7) 2_765 . . .
O1 P1 O2 Mo5 -176.8(5) 2_765 . . .
O1 P1 O2 Mo5 3.2(5) . . . .
O2 P1 O3 O2 180.002(2) . . . 2_765
O4 P1 O3 O2 -123.1(7) . . . 2_765
O4 P1 O3 O2 56.9(7) 2_765 . . 2_765
O1 P1 O3 O2 -60.2(6) 2_765 . . 2_765
O1 P1 O3 O2 119.8(6) . . . 2_765
O2 P1 O3 O4 -56.9(7) . . . .
O2 P1 O3 O4 123.1(7) 2_765 . . .
O4 P1 O3 O4 180.001(1) 2_765 . . .
O1 P1 O3 O4 62.9(7) 2_765 . . .
O1 P1 O3 O4 -117.1(7) . . . .
O2 P1 O3 O1 60.2(6) . . . .
O2 P1 O3 O1 -119.8(6) 2_765 . . .
O4 P1 O3 O1 117.1(7) . . . .
O4 P1 O3 O1 -62.9(7) 2_765 . . .
O1 P1 O3 O1 179.999(2) 2_765 . . .
O2 P1 O3 Mo3 177.1(6) . . . 2_765
O2 P1 O3 Mo3 -2.9(6) 2_765 . . 2_765
O4 P1 O3 Mo3 -125.9(8) . . . 2_765
O4 P1 O3 Mo3 54.1(8) 2_765 . . 2_765
O1 P1 O3 Mo3 -63.1(8) 2_765 . . 2_765
O1 P1 O3 Mo3 116.9(8) . . . 2_765
O2 P1 O3 Mo2 -53.0(8) . . . .
O2 P1 O3 Mo2 127.0(8) 2_765 . . .
O4 P1 O3 Mo2 4.0(6) . . . .
O4 P1 O3 Mo2 -176.0(6) 2_765 . . .
O1 P1 O3 Mo2 66.9(8) 2_765 . . .
O1 P1 O3 Mo2 -113.1(8) . . . .
Mo5 O1 O3 P1 -104.2(8) . . . .
Mo4 O1 O3 P1 103.9(7) 2_765 . . .
Mo6 O1 O3 P1 -179.5(5) . . . .
P1 O1 O3 O2 -46.1(5) . . . 2_765
Mo5 O1 O3 O2 -150.3(7) . . . 2_765
Mo4 O1 O3 O2 57.8(8) 2_765 . . 2_765
Mo6 O1 O3 O2 134.4(6) . . . 2_765
P1 O1 O3 O4 47.4(5) . . . .
Mo5 O1 O3 O4 -56.8(9) . . . .
Mo4 O1 O3 O4 151.3(7) 2_765 . . .
Mo6 O1 O3 O4 -132.1(6) . . . .
P1 O1 O3 Mo3 -112.4(8) . . . 2_765
Mo5 O1 O3 Mo3 143.4(6) . . . 2_765
Mo4 O1 O3 Mo3 -8.5(12) 2_765 . . 2_765
Mo6 O1 O3 Mo3 68.1(7) . . . 2_765
P1 O1 O3 Mo2 109.7(7) . . . .
Mo5 O1 O3 Mo2 5.5(11) . . . .
Mo4 O1 O3 Mo2 -146.4(5) 2_765 . . .
Mo6 O1 O3 Mo2 -69.8(6) . . . .
O3 P1 O4 O2 -124.0(7) . . . .
O3 P1 O4 O2 56.0(7) 2_765 . . .
O2 P1 O4 O2 180.000(1) 2_765 . . .
O1 P1 O4 O2 116.6(6) 2_765 . . .
O1 P1 O4 O2 -63.4(6) . . . .
O3 P1 O4 O3 180.000(1) 2_765 . . .
O2 P1 O4 O3 124.0(7) . . . .
O2 P1 O4 O3 -56.0(7) 2_765 . . .
O1 P1 O4 O3 -119.5(6) 2_765 . . .
O1 P1 O4 O3 60.5(6) . . . .
O3 P1 O4 Mo2 -4.2(6) . . . .
O3 P1 O4 Mo2 175.8(6) 2_765 . . .
O2 P1 O4 Mo2 119.8(8) . . . .
O2 P1 O4 Mo2 -60.2(8) 2_765 . . .
O1 P1 O4 Mo2 -123.6(8) 2_765 . . .
O1 P1 O4 Mo2 56.4(8) . . . .
O3 P1 O4 Mo1 -124.6(8) . . . .
O3 P1 O4 Mo1 55.4(8) 2_765 . . .
O2 P1 O4 Mo1 -0.6(6) . . . .
O2 P1 O4 Mo1 179.4(6) 2_765 . . .
O1 P1 O4 Mo1 116.0(7) 2_765 . . .
O1 P1 O4 Mo1 -64.0(7) . . . .
O3 P1 O4 Mo4 122.2(8) . . . .
O3 P1 O4 Mo4 -57.8(8) 2_765 . . .
O2 P1 O4 Mo4 -113.8(7) . . . .
O2 P1 O4 Mo4 66.2(7) 2_765 . . .
O1 P1 O4 Mo4 2.7(6) 2_765 . . .
O1 P1 O4 Mo4 -177.3(6) . . . .
O3 O2 O4 P1 -44.3(5) 2_765 . . .
Mo3 O2 O4 P1 -110.4(8) . . . .
Mo5 O2 O4 P1 107.9(7) . . . .
P1 O2 O4 O3 -42.1(5) . . . .
O3 O2 O4 O3 -86.4(7) 2_765 . . .
Mo3 O2 O4 O3 -152.5(7) . . . .
Mo5 O2 O4 O3 65.8(8) . . . .
P1 O2 O4 Mo2 -107.8(8) . . . .
O3 O2 O4 Mo2 -152.1(7) 2_765 . . .
Mo3 O2 O4 Mo2 141.8(6) . . . .
Mo5 O2 O4 Mo2 0.1(12) . . . .
P1 O2 O4 Mo1 179.5(5) . . . .
O3 O2 O4 Mo1 135.2(6) 2_765 . . .
Mo3 O2 O4 Mo1 69.1(7) . . . .
Mo5 O2 O4 Mo1 -72.6(6) . . . .
P1 O2 O4 Mo4 105.8(7) . . . .
O3 O2 O4 Mo4 61.4(8) 2_765 . . .
Mo3 O2 O4 Mo4 -4.7(12) . . . .
Mo5 O2 O4 Mo4 -146.4(5) . . . .
O2 O3 O4 P1 44.2(5) 2_765 . . .
O1 O3 O4 P1 -48.2(5) . . . .
Mo3 O3 O4 P1 108.9(9) 2_765 . . .
Mo2 O3 O4 P1 -176.4(5) . . . .
P1 O3 O4 O2 42.4(5) . . . .
O2 O3 O4 O2 86.6(7) 2_765 . . .
O1 O3 O4 O2 -5.8(7) . . . .
Mo3 O3 O4 O2 151.3(8) 2_765 . . .
Mo2 O3 O4 O2 -134.0(6) . . . .
P1 O3 O4 Mo2 176.4(5) . . . .
O2 O3 O4 Mo2 -139.4(6) 2_765 . . .
O1 O3 O4 Mo2 128.2(6) . . . .
Mo3 O3 O4 Mo2 -74.7(8) 2_765 . . .
P1 O3 O4 Mo1 105.7(9) . . . .
O2 O3 O4 Mo1 149.9(8) 2_765 . . .
O1 O3 O4 Mo1 57.5(10) . . . .
Mo3 O3 O4 Mo1 -145.4(7) 2_765 . . .
Mo2 O3 O4 Mo1 -70.7(7) . . . .
P1 O3 O4 Mo4 -101.8(8) . . . .
O2 O3 O4 Mo4 -57.6(9) 2_765 . . .
O1 O3 O4 Mo4 -150.0(7) . . . .
Mo3 O3 O4 Mo4 7.1(14) 2_765 . . .
Mo2 O3 O4 Mo4 81.8(7) . . . .
O9 Mo3 O5 Mo1 157.2(7) . . . .
O8 Mo3 O5 Mo1 -99.0(8) . . . .
O14 Mo3 O5 Mo1 1.4(13) 2_765 . . .
O18 Mo3 O5 Mo1 56.6(7) . . . .
O3 Mo3 O5 Mo1 -31.8(8) 2_765 . . .
O2 Mo3 O5 Mo1 -4.5(7) . . . .
V1 Mo3 O5 Mo1 42.6(9) 2_765 . . .
O16 Mo2 O6 Mo6 -159.6(8) . . . .
O12 Mo2 O6 Mo6 96.2(8) . . . .
O17 Mo2 O6 Mo6 -7.4(14) . . . .
O14 Mo2 O6 Mo6 -58.7(8) . . . .
O4 Mo2 O6 Mo6 30.9(8) . . . .
O3 Mo2 O6 Mo6 1.7(7) . . . .
V1 Mo2 O6 Mo6 -45.0(10) . . . .
O9 Mo3 O8 Mo6 -158.1(7) . . . 2_765
O5 Mo3 O8 Mo6 99.5(8) . . . 2_765
O14 Mo3 O8 Mo6 -55.5(8) 2_765 . . 2_765
O18 Mo3 O8 Mo6 1.5(14) . . . 2_765
O3 Mo3 O8 Mo6 5.2(7) 2_765 . . 2_765
O2 Mo3 O8 Mo6 33.3(8) . . . 2_765
V1 Mo3 O8 Mo6 -41.5(9) 2_765 . . 2_765
O16 Mo2 O12 Mo1 158.9(8) . . . .
O6 Mo2 O12 Mo1 -98.1(8) . . . .
O17 Mo2 O12 Mo1 56.1(8) . . . .
O14 Mo2 O12 Mo1 4.0(14) . . . .
O4 Mo2 O12 Mo1 -4.2(7) . . . .
O3 Mo2 O12 Mo1 -31.5(8) . . . .
V1 Mo2 O12 Mo1 42.6(9) . . . .
O7 Mo5 O13 Mo1 -162.4(7) . . . .
O22 Mo5 O13 Mo1 94.8(8) . . . .
O19 Mo5 O13 Mo1 -9.8(15) 2_765 . . .
O18 Mo5 O13 Mo1 -61.3(8) . . . .
O1 Mo5 O13 Mo1 30.1(8) . . . .
O2 Mo5 O13 Mo1 0.1(7) . . . .
V1 Mo5 O13 Mo1 -48.3(10) 2_765 . . .
O20 Mo4 O21 Mo6 153.4(9) . . . 2_765
O23 Mo4 O21 Mo6 -101.3(10) . . . 2_765
O17 Mo4 O21 Mo6 -2.0(17) . . . 2_765
O19 Mo4 O21 Mo6 54.1(10) . . . 2_765
O1 Mo4 O21 Mo6 -5.1(8) 2_765 . . 2_765
O4 Mo4 O21 Mo6 -35.8(10) . . . 2_765
V1 Mo4 O21 Mo6 39.9(12) . . . 2_765
O7 Mo5 O22 Mo6 156.7(8) . . . .
O13 Mo5 O22 Mo6 -100.9(8) . . . .
O19 Mo5 O22 Mo6 55.5(8) 2_765 . . .
O18 Mo5 O22 Mo6 -0.9(15) . . . .
O1 Mo5 O22 Mo6 -4.5(7) . . . .
O2 Mo5 O22 Mo6 -33.9(9) . . . .
V1 Mo5 O22 Mo6 41.5(10) 2_765 . . .
O20 Mo4 O23 Mo1 -156.0(9) . . . .
O21 Mo4 O23 Mo1 100.6(10) . . . .
O17 Mo4 O23 Mo1 -53.7(10) . . . .
O19 Mo4 O23 Mo1 4.6(17) . . . .
O1 Mo4 O23 Mo1 36.8(10) 2_765 . . .
O4 Mo4 O23 Mo1 5.0(8) . . . .
V1 Mo4 O23 Mo1 -39.7(12) . . . .
C14 C13 C12 C11 -2.4(15) . . . .
C13 C13 C12 C11 176.0(11) 2_776 . . .
C13 C12 C11 N3 0.9(16) . . . .
C15 N3 C11 C12 1.2(16) . . . .
Cu2 N3 C11 C12 -176.7(9) 2_766 . . .
Cu2 N3 C11 C12 -174.6(9) . . . .
C11 N3 C15 C14 -1.6(17) . . . .
Cu2 N3 C15 C14 175.9(10) 2_766 . . .
Cu2 N3 C15 C14 174.8(10) . . . .
N3 C15 C14 C13 0.0(19) . . . .
C12 C13 C14 C15 2.0(16) . . . .
C13 C13 C14 C15 -176.4(12) 2_776 . . .
C18 N4 C16 C21 137.8(12) . . . .
C19 N4 C16 C21 84(2) . . . .
C17 N4 C16 C21 160.8(15) . . . .
C20 N4 C16 C21 16.6(13) . . . .
C21 N4 C16 C17 -160.8(15) . . . .
C18 N4 C16 C17 -23.0(13) . . . .
C19 N4 C16 C17 -77(2) . . . .
C20 N4 C16 C17 -144.2(11) . . . .
C21 N4 C16 C19 -75.8(16) . . . 2_655
C18 N4 C16 C19 62.0(18) . . . 2_655
C19 N4 C16 C19 8(3) . . . 2_655
C17 N4 C16 C19 84.9(17) . . . 2_655
C20 N4 C16 C19 -59.2(17) . . . 2_655
C21 N4 C16 C18 -43.5(10) . . . 2_655
C18 N4 C16 C18 94.4(11) . . . 2_655
C19 N4 C16 C18 40(2) . . . 2_655
C17 N4 C16 C18 117.3(13) . . . 2_655
C20 N4 C16 C18 -26.9(11) . . . 2_655
C21 C16 C17 C18 4(2) . . . .
N4 C16 C17 C18 23.4(13) . . . .
C19 C16 C17 C18 -87.4(17) 2_655 . . .
C18 C16 C17 C18 -51(2) 2_655 . . .
C21 C16 C17 N4 -19.3(15) . . . .
C19 C16 C17 N4 -110.9(13) 2_655 . . .
C18 C16 C17 N4 -74.3(12) 2_655 . . .
C21 C16 C17 C20 90.4(19) . . . 2_655
N4 C16 C17 C20 109.7(13) . . . 2_655
C19 C16 C17 C20 -1.1(15) 2_655 . . 2_655
C18 C16 C17 C20 35.4(16) 2_655 . . 2_655
C21 N4 C17 C16 17.3(14) . . . .
C18 N4 C17 C16 154.9(14) . . . .
C19 N4 C17 C16 140.1(13) . . . .
C20 N4 C17 C16 71(2) . . . .
C21 N4 C17 C18 -137.6(12) . . . .
C19 N4 C17 C18 -14.8(13) . . . .
C16 N4 C17 C18 -154.9(14) . . . .
C20 N4 C17 C18 -83(2) . . . .
C21 N4 C17 C20 -62.7(17) . . . 2_655
C18 N4 C17 C20 74.9(15) . . . 2_655
C19 N4 C17 C20 60.1(17) . . . 2_655
C16 N4 C17 C20 -80.0(16) . . . 2_655
C20 N4 C17 C20 -9(3) . . . 2_655
C21 N4 C18 C19 -76(2) . . . .
C16 N4 C18 C19 -139.5(13) . . . .
C17 N4 C18 C19 -161.9(15) . . . .
C20 N4 C18 C19 -21.0(14) . . . .
C21 N4 C18 C17 86(2) . . . .
C19 N4 C18 C17 161.9(15) . . . .
C16 N4 C18 C17 22.4(13) . . . .
C20 N4 C18 C17 140.9(11) . . . .
C21 N4 C18 C21 9(3) . . . 2_655
C19 N4 C18 C21 84.9(17) . . . 2_655
C16 N4 C18 C21 -54.5(18) . . . 2_655
C17 N4 C18 C21 -77.0(16) . . . 2_655
C20 N4 C18 C21 63.9(17) . . . 2_655
C21 N4 C18 C16 -30(2) . . . 2_655
C19 N4 C18 C16 45.5(11) . . . 2_655
C16 N4 C18 C16 -94.0(12) . . . 2_655
C17 N4 C18 C16 -116.4(12) . . . 2_655
C20 N4 C18 C16 24.5(12) . . . 2_655
C16 C17 C18 C19 -4(3) . . . .
N4 C17 C18 C19 20.3(17) . . . .
C20 C17 C18 C19 -92(2) 2_655 . . .
C16 C17 C18 N4 -23.9(13) . . . .
C20 C17 C18 N4 -112.4(11) 2_655 . . .
C16 C17 C18 C21 88.3(16) . . . 2_655
N4 C17 C18 C21 112.2(11) . . . 2_655
C20 C17 C18 C21 -0.2(12) 2_655 . . 2_655
C16 C17 C18 C16 50(2) . . . 2_655
N4 C17 C18 C16 74.3(11) . . . 2_655
C20 C17 C18 C16 -38.2(14) 2_655 . . 2_655
C17 C18 C19 N4 -19.8(16) . . . .
C21 C18 C19 N4 -108.8(13) 2_655 . . .
C16 C18 C19 N4 -108.7(13) 2_655 . . .
N4 C18 C19 C16 108.7(13) . . . 2_655
C17 C18 C19 C16 89(2) . . . 2_655
C21 C18 C19 C16 0.0(16) 2_655 . . 2_655
N4 C18 C19 C20 21.8(14) . . . .
C17 C18 C19 C20 2(3) . . . .
C21 C18 C19 C20 -87.0(18) 2_655 . . .
C16 C18 C19 C20 -87.0(18) 2_655 . . .
C21 N4 C19 C18 139.1(13) . . . .
C16 N4 C19 C18 75(2) . . . .
C17 N4 C19 C18 16.2(14) . . . .
C20 N4 C19 C18 157.9(14) . . . .
C21 N4 C19 C16 56.1(17) . . . 2_655
C18 N4 C19 C16 -83.0(17) . . . 2_655
C16 N4 C19 C16 -8(3) . . . 2_655
C17 N4 C19 C16 -66.8(17) . . . 2_655
C20 N4 C19 C16 75.0(15) . . . 2_655
C21 N4 C19 C20 -18.8(12) . . . .
C18 N4 C19 C20 -157.9(14) . . . .
C16 N4 C19 C20 -83(2) . . . .
C17 N4 C19 C20 -141.7(11) . . . .
C18 N4 C20 C21 -139.2(13) . . . .
C19 N4 C20 C21 -157.5(14) . . . .
C16 N4 C20 C21 -17.8(13) . . . .
C17 N4 C20 C21 -74(2) . . . .
C21 N4 C20 C17 82.2(16) . . . 2_655
C18 N4 C20 C17 -56.9(17) . . . 2_655
C19 N4 C20 C17 -75.3(15) . . . 2_655
C16 N4 C20 C17 64.5(16) . . . 2_655
C17 N4 C20 C17 9(3) . . . 2_655
C21 N4 C20 C19 157.5(14) . . . .
C18 N4 C20 C19 18.3(12) . . . .
C16 N4 C20 C19 139.7(12) . . . .
C17 N4 C20 C19 84(2) . . . .
C18 C19 C20 C21 -1(2) . . . .
N4 C19 C20 C21 21.8(14) . . . .
C16 C19 C20 C21 -90.9(17) 2_655 . . .
C18 C19 C20 N4 -22.5(15) . . . .
C16 C19 C20 N4 -112.7(13) 2_655 . . .
C18 C19 C20 C17 91.2(19) . . . 2_655
N4 C19 C20 C17 113.7(12) . . . 2_655
C16 C19 C20 C17 1.0(14) 2_655 . . 2_655
N4 C20 C21 C16 22.4(17) . . . .
C17 C20 C21 C16 -88(2) 2_655 . . .
C19 C20 C21 C16 2(3) . . . .
C17 C20 C21 N4 -110.2(11) 2_655 . . .
C19 C20 C21 N4 -20.9(13) . . . .
N4 C20 C21 C18 110.4(11) . . . 2_655
C17 C20 C21 C18 0.3(13) 2_655 . . 2_655
C19 C20 C21 C18 89.6(16) . . . 2_655
C17 C16 C21 C20 -3(3) . . . .
N4 C16 C21 C20 -23.2(17) . . . .
C19 C16 C21 C20 92(2) 2_655 . . .
C18 C16 C21 C20 92(2) 2_655 . . .
C17 C16 C21 N4 19.8(15) . . . .
C19 C16 C21 N4 115.0(13) 2_655 . . .
C18 C16 C21 N4 115.0(13) 2_655 . . .
C17 C16 C21 C18 -95.2(19) . . . 2_655
N4 C16 C21 C18 -115.0(13) . . . 2_655
C19 C16 C21 C18 0.0(14) 2_655 . . 2_655
C18 N4 C21 C20 76(2) . . . .
C19 N4 C21 C20 21.5(14) . . . .
C16 N4 C21 C20 159.6(15) . . . .
C17 N4 C21 C20 142.4(12) . . . .
C18 N4 C21 C16 -84(2) . . . .
C19 N4 C21 C16 -138.1(13) . . . .
C17 N4 C21 C16 -17.2(14) . . . .
C20 N4 C21 C16 -159.6(15) . . . .
C18 N4 C21 C18 -9(3) . . . 2_655
C19 N4 C21 C18 -63.7(18) . . . 2_655
C16 N4 C21 C18 74.5(16) . . . 2_655
C17 N4 C21 C18 57.2(19) . . . 2_655
C20 N4 C21 C18 -85.1(17) . . . 2_655
